**P-70.1 **

**OBERST BEAM AS A TOOL FOR COMPLEX YOUNG’S MODULUS **

**MEASUREMENT OF POROUS MATERIALS. **

PACS: 43.40.AtExperimental and theoretical studies of vibrating systems

O. Danilov; F. Sgard; X. Olny

LASH/DGCB URA CNRS 1652, Ecole Nationale des Travaux Publics de l'Etat Rue Maurice Audin, 69518

Vaulx-en-Velin Cedex France

Tel: +33 4 72 04 70 36 Fax:+33 4 72 04 70 41 E-mail: danilov@entpe.fr

**ABSTRACT**

The prediction of the vibroacoustic performance of systems including porous materials requires a correct estimation of the mechanical parameters of porous materials. This paper investigates the adaptation of Oberst beam method developed for viscoelastic materials to the determination of complex Young’s modulus of porous materials. Analytical and numerical results based on a finite element model show that there are some special conditions including dimensions of test sample and boundary conditions where porous materials behave as viscoelastic ones. It is then possible to determine the complex Young’s modulus according to this method. For these configurations, acceptable experimental results are obtained in the case of different foamed and fibrous materials.

**1. INTRODUCTION**

Porous materials are often used as passive elements of noise reduction systems. Mainly used for sound absorbing purposes porous materials have also an ability to damp vibrations of mechanical structures. Being integrated into a multifunctional noiseproofing part, a porous material can reduce appreciably the vibration levels of, for example, steel car body panels. Among the parameters of porous materials, the complex Young’s modulus of skeleton influences strongly the damping behaviour of the porous media, and several methods exist for its determination [1], [2]. However, considering the porous material mainly as a damper, it is interesting to examine the application to porous material of a test method especially developed for damping material, such as Oberst’s beam method.

**2. THEORY: COMPLEX YOUNG’S MODULUS DETERMINATION **

Oberst’s beam consists of a material to be tested bonded onto a metal slice, which is clamped at one end and excited at the other end (see figure 1).

Porous layer

Metal beam

Excitation

Clamp Laser vibration transducer

*Figure 1: Oberst beam *

Before dealing with the theoretical background of the proposed method it is important to recall the main assumptions made:

Ø the test sample is considered as a rod-like one, i.e. its deformations are extensional-compressional and are controlled by complex Young’s modulus without any influence of Poisson ratio (a);

Ø the dimensions of the test sample and the frequency range of measurements suppose a viscoelastic dynamic behaviour of a porous material (b);

Ø the porous material behaves in a linear way in the frequency range and deformation amplitudes of interest (c);

Ø angle of deformation of porous layer does not change with thickness that means the angle is the same in lower layer and in upper layer of porous material as it is shown on figure 2 (d);

Ø in the resonance zone, the variation of Young’s modulus and loss factor vs. frequency is negligible (e).

Neutral axis of layer 1 Neutral axis of layer 2

*x*

*H*

_{0}*H*

_{2}*H*

_{02}* y*

### Neutral plane of

### bending

### Porous layer

### Elastic layer

*θ*

*ξ*

*y*

_{ξ}*H*

_{01}*H*

_{1}*Figure 2: Deformed and undeformed composite beam *

Briefly, the Young’s modulus determination by this method is based on the comparison of the natural frequencies of the bare beam and the composite beam (metal beam with porous layer). The natural frequency of the homogenous beam is given by

4 2

0

*b*
*b*

*b*
*n*
*n*

*L*

*m*

*B*

*f*

### =

*ξ*

, (1)
where
*n* is the mode index,

*ξ*

*n*is the mode coefficient,

*B _{b}* is the bending stiffness of the beam,

*L _{b}* is the length of the beam.

It can be shown [4], after comparison of the bending moments with respect to neutral plane of
bending of composite beam with the bending moment with respect to horizontal axis *x* (see
figure 2), that the Young’s moduli of the substrate and of the material are linked to each other by
the following equation

02

01 1 1 2

1 1 2

*I*

*I*

*I*

*m*

*m*

*E*

*E*

*c*

*c*

### ⋅

### −

###

###

###

###

### ⋅

### =

*ω*

*ω*

, (2)

where

2 1

### ,

*E*

*E*

are the Young’s moduli of steel substrate and porous layer, respectively,
*ω*

*c*is the natural frequency of the two-layer beam,

*ω*

1 is the natural frequency of the steel substrate alone,
*I1*

is the moment of inertia per unit length of the steel substrate *I*

_{1}

*H*1 3

12

### =

,02 01

### ,

*I*

*I*

are the moments of inertia per unit length relative to the neutral plane of
bending of the composite beam,
1

*m*

is the mass per unit length per unit width of the steel substrate, *m*

_{1}

### =

*ρ*

_{1}

*H*

_{1}, where

*ρ*

1 denotes the density of steel, and *H*1 denotes its thickness,

*c*

*m*

is the mass per unit length per unit width of the composite beam,
2 2 1

1

*H*

*H*

*m*

_{c}### =

*ρ*

### +

*ρ*

, where *ρ*

_{2}denotes the density of the porous layer, and

*H*

_{2}

denotes its thickness.

It is necessary to note that equation (2) supposes a linear deformation of the porous layer as it is supposed by assumption (d).

Although the Young’s modulus of the porous material can be obtained directly, from the classical Oberst’s beam approach, the assessment of the loss factor is not as straight founded. Indeed, classical Oberst’s beam theory supposes the loss factor of the bare steel slice is negligible in comparison with the loss factor of the composite beam. In the case of the composite beam involving a porous layer, the loss factor of this composite beam may not be very large. The porous layer does not change strongly the dynamic behaviour of the beam due to a low specific weight and a low Young’s modulus of the skeleton. This feature requires to a modification the technique in order to take in account the loss factor of the metal substrate.

The length of the paper does not allow one to present a complete derivation of the loss factor
expression. Therefore only the most important steps and assumptions will be presented. The
loss factor is defined as the ratio of the energy dissipated per cycle of oscillations (*D)* to the
potential energy (*U)* of the system (or structure). In general, the energy of the two- (or multi)
layer structures can be described as a sum of the energies stored and dissipated in each layer.
The damping action of a multi-layer structure is considered as a set of springs, where each
spring represents a storing energy mechanism. The displacement of the first layer (bending
deformation of a beam to be damped) causes a displacement of the second one. The energy
stored in one spring is *W _{i}*

### =

*K*

_{i}### ⋅

*x*2

_{i}, where *K _{i}*is the stiffness of the spring, and

*x*its strain. In case of periodic displacement, the energy dissipated per cycle of oscillation, is

_{i}*D*

_{i}### =

2*πη*

*, so that the loss factor of the multilayer structure is given by:*

_{i}W_{i}*η*

*π*

*π*

*η*

*η*

### =

### ⋅

### =

### =

### =

### ∑

### ∑

### ∑

### ∑

### ∑

### ∑

*D*

*U*

*D*

*W*

*W*

*W*

*K x*

*K x*

*i*
*i*

*i*
*i*

*i* *i*
*i*

*i*
*i*

*i* *i* *i*
*i*

*i* *i*
*i*

2 2

2

2 , (3)

mechanism one may conclude that the value of

*K*

*ext*is determined by the bending stiffness of

each layer, and by the extensional deformations of both layers. On the basis of energy equations, shown in [7], it is possible to write for one layer

2 2 2

### 2

### 1

### 2

### 1

*dx*

*d*

*B*

*K*

*w*

*w*

*x*

*K*

_{ext}

_{ext}### =

_{ext}### +

_{flex}### =

### ⋅

*ε*

### +

*θ*

(4)
where *K*

### =

*E*

### ⋅

*A*

is an extensional stiffness, *A*

is the cross-section area;
*dx*

*d*

*ξ*

*ε*

### =

, where*ξ*

is the mean axial displacement of an element of material, *x*

is the
horizontal coordinate, *B*

is the bending stiffness of the layer relatively to the neutral
plane of bending, *θ*

is the bending angle.
Figure 2 shows the displacements in the system. In order to simplify the model, it is assumed that because of the small value of

*θ*

the axial displacement *ξ*

is taken as equal to the
displacement along the *x*-axis. In other words, one assumes the absence any shear deformation into the porous layer. Thus, the following relation holds:

*θ*

*θ*

*ξ*

### =

*y*

_{ξ}### ⋅

### tan

### ≡

*y*

_{ξ}### ⋅

, (5) where*y*

*denotes on figure 2. Thus, taking into account that*

_{ξ}## (

## )

*dx*

*d*

*y*

*y*

*dx*

*d*

*dx*

*d*

*ξ*

_{θ}

_{θ}

*θ*

*ε*

### =

### =

*ξ*

### ⋅

### =

*ξ*

### ⋅

,equation (3) can be rewritten as

## (

## )

## (

## )

## (

## )

## (

## )

## (

## )

## (

## )

### ∑

### ∑

### ∑

### ∑

= = = =### +

### +

### =

### +

###

###

###

###

###

###

### +

###

###

###

###

###

###

### =

_{2}1 2 2 1 2 2 1 2 2 2 1 2 2

### 2

### 1

### 2

### 1

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*i*

*ext*

*c*

*B*

*y*

*h*

*E*

*B*

*y*

*h*

*E*

*B*

*y*

*h*

*E*

*dx*

*d*

*B*

*y*

*h*

*E*

*dx*

*d*

*ξ*

*ξ*

*ξ*

*ξ*

*η*

*θ*

*η*

*θ*

*η*

, (6)
where

*B*

*is the bending stiffness of the layer*

_{i}*i*relatively to the neutral plane of bending,

*i*
*i*
*i*

*h*

*E*

### ,

### ,

*η*

are the Young’s modulus, thickness, and loss factor of layer *i*

, respectively,
and *y*

*are determined from geometrical relationships shown on figure 2.*

_{ξ}_{i}Equation (6) establishes the relationship between the loss factor of the composite beam (

*η*

*), the loss factor of the bare steel slice (*

_{c}_{ext}*η*

_{1}), which need to be measured, and the loss factor (

*η*

_{2}) of the porous layer, which is the objective of the measurement. The loss factor

*η*

_{2}can then be calculated from the following:

## (

## ) (

## )

2 2 2 2 2 1 2 1 1 1 1 2 1 2 2*B*

*y*

*h*

*E*

*B*

*y*

*h*

*E*

*B*

*y*

*h*

*E*

*i*

*i*

*i*

*i*

*i*

*ext*

*c*

### +

### +

### −

### +

### =

### ∑

=*ξ*

*ξ*

*ξ*

*η*

*η*

*η*

, (7)
Thus, equations (2) and (7) allow one to calculate the Young’s modulus and the loss factor of
porous layer.
**3. EXPERIMENTAL RESULTS AND FINITE-ELEMENT MODELLING: DISCUSSION **
**OF THE LIMITATION OF THE PRESENTED APPROACH**

*Figure 3: Example of measured frequency response function *

Table 1 shows

### E

a and ηa (apparent Young’s modulus and loss factor), which have been determined using equations (2) and (7) for the second natural mode of the beam. The values of Young’s moduli indicated on the first line have been obtained by numerous measurements based on the resonance test method and are considered as a reference.Table 1. Foam 1: ρ=28 kg/m3;

Emod=118 kPa, η=0.125

Foam 2: ρ=8.4 kg/m3; Emod=530 kPa, η=0.09

Fibrous: ρ=63 kg/m3; Emod=116 kPa, η=0.30 T, mm Fres, Hz Ea,

kPa

ηa T, mm Fres, Hz

Ea, kPa

ηa T, mm Fres, Hz Ea, kPa

ηa

27 168.1 70 0.14 27 199.3 188 0.09 15 164.4 113 0.13 20 189 310 0.09 10 164.16 115 0.12

5 165.7 119 0.12

10 172.4 535 0.08

10 158.3 120 0.35

*Figure 4: Finite-element modelling: *
*displacements of cross-section of *

*composite beam *

The picture illustrates the change of the bending angle along the thickness. It shows that upper layers of porous material bend more strongly than lower ones. In the case of low thicknesses of porous layer (5…15 mm), finite-element (FE) simulations show that the bending angle remains constant in the thickness of the porous material. It is confirmed by finite-element simulations shown in table 2.

Table 2.

Foam 1: ρ=28 kg/m3; Emod=118 kPa Foam 2: ρ=8.4 kg/m3; Emod=530 kPa Thickness of

porous layer, mm

Resonance frequency, FE

simulation

Resonance frequency, analytical

prediction by equation (2)

Resonance frequency, FE

simulation

Resonance frequency, analytical prediction

by equation (2)

0 168.1 168.2 168.1 168.2

5 165.7 165.9 167.9 168.1

10 163.6 164.3 170.8 172.2

15 162.1 164.5 176.1 183.8

20 161.1 167.0 185.3 205.0

27 160.6 175.5 201.7 251.9

One can conclude that in the case of both materials a good agreement between analytically and numerically predicted frequencies is observed at thicknesses of porous materials equal to 5 and 10 mm. Very similar results have been obtained experimentally (see table 1). Thus, one can say that for porous materials with Young’s modulus ranging from 100 to 500 kPa, the thickness of the porous layer should be limited to 10 mm if Oberst’s beam is to be used. On the other hand, it is necessary to point out that this limitation is related to the assumptions made in the derivation of the analytical formula for Young’s modulus calculation. This is not a limitation inherent to Oberst’s beam method, which could use numerical FE calculation.

**4. CONCLUSIONS**

Oberst’s beam method has been adapted to determine complex Young’s moduli of porous materials. The modified equations of loss factor determination and one principal limit of the method have been established. The experimental results obtained by the proposed method for three different materials showed a good agreement with the ones received by an other test method.

**5. ACKNOWLEDGEMENTS**

This research was supported by Region Rhône-Alpes in the framework of research project IMPACT.

**REFERENCES**

[1] E. Mariez, S. Sahraou, J.F. Allard “Elastic constants of polyurethane foam’s skeleton for Biot model,” Proceedings of INTER-NOISE 96, 951-954.

[2] C. Langlois, R. Panneton, N. Attala, “A method for the mechanical characterisation of poroelastic materials,” Canadian Acoustics/Acoustique canadienne, v. 28 No. 3, 82-83 (2000).

[3] H. Oberst, K. Frankenfeld, “Uder die Dampfungder Biegeschwingungen dunner Bleche durch festhaftende Belage”, Acustica, 2, pp. 181-194, 1952.

[4] L. Mina, Liu Guo Liang, L. Garibaldi. “The Estimation of Damping Material Loss Factor in the Oberst Beam Test”. 2nd International Conference VEHICLE COMFORT, Vol. 1, pp. 197-205, Bologna, Italy, 1992.

[5] P.Saha, J. Cahine “The Testing of Vibration Damping Materials”. Sound and Vibration. May, 1995, pp. 38-45

[6] Rapport de recherche, année 2, contrat Région Rhône-Alpes IMPACT (Innovation en Mécanique Passive et Active pour la Prévision et le Contrôle vibroacoustique), 2002.